Mechanisms of Microstructure Control in Conventional Sintering spark plasma sintering (Gao et al.,...
Embed Size (px)
Transcript of Mechanisms of Microstructure Control in Conventional Sintering spark plasma sintering (Gao et al.,...
Mechanisms of Microstructure Control in Conventional Sintering
Adriana Scoton Antonio Chinelatto1, Elíria Maria de Jesus Agnolon Pallone2,
Ana Maria de Souza1, Milena Kowalczuk Manosso1, Adilson Luiz Chinelatto1 and Roberto Tomasi3
1Department of Materials Engineering - State University of Ponta Grossa 2Department of Basic Sciences – FZEA - São Paulo University
3Department of Materials Engineering - Federal University of São Carlos Brazil
The manner and mechanisms involved on the sintering process are essential investigation to achieve the required microstructure and final properties in solids. During the conventional sintering of a compacted powder, densification and grain growth occur simultaneously through atomic diffusion mechanisms. Many researchers have been working on reducing
the grain size below 1 µm aiming to improve some properties, such as strength, toughness and wear resistance in ceramics (Greer, 1998; Inoue & Masumoto, 1993; Morris, 1998). In order to obtain ultra-fine ceramic microstructures, nanocrystalline powders can be used. Although the sinterability of nanoparticles is superior to that of fine particles due to the higher sintering stress, densification of these powders is often accompanied by grain growth (Suryanarayana, 1995).
Hot pressing sintering (He & Ma, 2000; Porat et al., 1996), spark plasma sintering (Gao et al., 2000; Chakravarty et al., 2008) or pulse electric current sintering (Zhou et al., 2004) are typical techniques employed to produce nanostructured ceramics. However, many of these techniques are not economically viable depending on the use of the final product. Thus, conventional pressureless sintering is still a more attractive sintering method to produce ceramic products, mainly due to its simplicity and cost compared to other methods. In the conventional pressureless sintering, a controlled grain size with high densification could be achieved by adequate control procedures of the heating curve — herein defined as the maximization of the final density with minimum grain growth.
One hypothesis to the heating curve control can be achieved by improving the narrowing of grain size distribution in a pre-densification sintering stage followed by a final densification stage namely at a maximum densification rate temperature (Chu et al., 1991; Lin & DeJonghe, 1997a, 1997b). In a thermodynamics point-of-view, another hypothesis is regarded to control the heating schedule at temperature ranging the active grain boundary diffusion. Note, however, that the grain boundary migration is sufficiently sluggish and the
Sintering of Ceramics – New Emerging Techniques
densification could occur without grain growth. The aforementioned hypothesis was proposed by Chen and Wang (Chen & Wang, 2000) and has been successfully applied to different types of materials. A second phase can be added to preserve fine grains. In this case, grain boundary inhibition can be due to the pinning effect, which is associated with particles locations at grain boundaries or triple junctions (Chaim e al. 1998; Trombini et al., 2007). This drag pinning effect associated with heating curve control can be more effective to suppress the grain growth.
2. Nanostructure materials
The size control of microstructural elements has been always considered as one of the most important factors in control of several properties in the development of new materials or design new microstructures. As a historical example, it can be mentioned that the grain refining of metallic materials, which results in increased mechanical strength, tenacity, occurrence of superplastic, etc. New materials with sub-micron grain size have been developed recently as commercial materials and the latest generation of this development is the nanostructured materials (Inoue & Masumoto, 1993).
Nanostructured materials (also called nanocrystalline materials, nanophasics materials or nanometer-sized crystalline solids) are known to have properties or combinations of properties, which may be new or even superior to conventional materials (Greer, 1998). Nanostructured materials can be defined as a system containing at least one microstructural nano characteristic (with sizes ranging up to 100-150nm). Due the extremely small dimensions, a large volume fractions atoms located in grain boundaries (Morris, 1998), which gives them a unique combination of composition and microstructure (Suryanarayana, 1995). Generally, these materials exhibit high strength and hardness, increased diffusivity, improved ductility and toughness, reduced elastic modulus, lower thermal conductivity
when compared to larger grain size materials (~10µm) (Suryanarayana, 1995).
Since nanocrystalline materials contain a large fraction of atoms in grain boundaries, many of these interfaces provide high density of short diffusion paths. Therefore, it is expected that these materials show increased diffusivity compared to polycrystalline materials of the same composition and conventional particle size (of the order of microns) (He & Ma, 2000). The consequence of such increased diffusivity is increased sinterability of nanometric powders, which causes decrease in sintering temperature of these powders when compared to the same material with conventional particle size (Porat et al., 1996).
The driving force for sintering or "sintering stress" of nanocrystalline ceramics with pores in the range of 5nm is about 400MPa (considering γ about 1Jm-2), while for conventional ceramics with pores around 1 µm it is 2 MPa. Thus, a nanocrystalline ceramic must have a great thermodynamic driving force for retraction, which must densify extremely well even under unfavorable kinetic conditions such as low temperatures (Suryanarayana, 1995).
The interest in this nanostructured materials area has grown due to the availability of nanocrystalline ceramic powders. These nanocrystalline powders can be synthesized using different techniques, but its consolidation into dense ceramics without significant grain growth is still a challenge.
Compaction and sintering of ultra fine and/or nanoscale powder have a positive set of aspects over behavior during processing and final properties of products; however, there are also
Mechanisms of Microstructure Control in Conventional Sintering
several processing difficulties. Main positive aspects include: increased reactivity between reagents and solid particles and between particles and the gas phase, which are important processes in synthesis; increased sintering rate and particularly lowering of sintering temperature, which can reduced by half the material’s melting point (Hahn, 1993; Mayo, 1996).
On the other hand, also due to the large surface area and large excess of free energy nanometric powder systems, there are many detrimental aspects to the processing and obtaining the refined and homogeneous microstructures. Some of these aspects are: a very strong tendency to agglomeration of primary particles of nanometric powders; difficulties of mixing and homogenization of compression due to the strong attraction between particles; demand for greater sintering atmosphere control, not only due to the higher reactivity, but also the possibility of formation of thermodynamically unstable phases and appearance of strong effect of adsorbed gases on the surface (Allen et al., 1996; Averback et al., 1992).
Many studies (Chen & Chen, 1996, 1997) on nanometric size particles have shown reduction of sintering temperature. Hahn et al. (Hanh, 1990), studying the sintering of nanometric TiO2 (12nm), Y2O3 (4 nm) and ZrO2 (8nm), found lower sintering temperatures than those conventional. The sintering of TiO2 occurred at 1000ºC while conventional TiO2 sintering requires temperatures above 1400ºC. The same pattern of reduced sintering temperature was observed for Y2O3 and ZrO2. In spite of the proven decrease in sintering temperature of nanometric powders, its densification is often accompanied by a large grain growth, causing lost of their nanocrystalline ceramics characteristics.
2.1 Effect of heating curve in the sintering
Production of polycrystalline ceramics with high density and small grain size have been studied for several processing routes. Among these routes may be cited: colloidal processes of powder with controlled particle size distribution (Sigmund & Bergström, 2000; Lim et al., 1997), sintering under pressure (He & Ma, 2000; Weibel et al.,1997), use of additives incorporated into a second phase or in solid solution (Novkov, 2006; Erkalfa et al., 1996), spark plasma sintering (Gao et al., 2000; Chakravarty et al., 2008, Bernard-Granger & Guizard, 2007), pulse electric current sintering (Zhou et al., 2004), etc. Usually these methods have several limitations on usage, in addition to requiring more complex and expensive equipment. Thus, sintering without pressure is even a more desirable sintering method to produce ceramic products, mainly due to its simplicity and cost when compared to other methods.
In pressureless sintering, beyond the control of powders’ characteristics, control of the sintering process has a major effect on final material’s density and microstructure. This method is often unable to prepare dense ceramics with ultrafine grain size, once way the final sintering stage, both densification and grain growth occur by the same diffusion mechanisms (Mazahery et al., 2009).
Heating curve control to manipulate the micro